## Phase Transition and Electronic Structure Investigation of MoS2-rGO

## Nanocomposite Decorated with AuNPs.

Yunier  Garcia-Basabe 1,* , Gabriela  F. Peixoto , 2 Daniel  Grasseschi 2,3 , Eric C. Romani 4 , Flávio  C.  Vicentin , 5 Cesar  E.  P.  Villegas ,  Alexandre.  R.  Rocha 6 7 and Dunieskys G. Larrude 3

1 Universidade Federal da Integração Latino-Americana, UNILA, 85867-970, Foz do Iguaçu, Brazil.

2 Inorganic  Chemistry  Department,  Chemistry  Institute,  Federal  University  of  Rio  de Janeiro (UFRJ), 21941-909, Rio de Janeiro, Brazil

3 MackGraphe-Graphene and Nanomaterial Research Center, Mackenzie Presbyterian University, 01302-907, São Paulo, Brasil.

4 SENAI  Innovation  Institute  for  Virtual  Production  Systems,  20911-210,  Rio  de Janeiro, Brazil.

5 Brazilian  Synchrotron  Light  Laboratory  (LNLS),  Brazilian  Center  for  Research  in Energy and Materials (CNPEM), 13083-970, Campinas, Sao Paulo, Brazil.

6 Departamento  de  Ciencias,  Universidad  Privada  del  Norte,  Av.  Andrés  Belaunde Cdra. 10 s/n, 15324, Comas, Lima, Peru .

7 Instituto de Física Teórica, State University of São Paulo (UNESP), 01049-010, São Paulo, Brazil.

*Corresponding Author:

Prof. Dr. Yunier Garcia-Basabe

E-mail address: yunier.basabe@unila.edu.br and yunierbasabe26@gmail.com

ORCID iD: 0000-0001-5683-0108

. Keywords : MoS2, Reduced graphene oxide, nanocomposite, phase transition, electronic structure, surface decoration, gold nanoparticles

## ABSTRACT

In  this  work  a  simple  approach  to  transform  MoS2  from  its  metallic  (1T'  to semiconductor  2H)  character  via  gold  nanoparticle  surface  decoration  of  a  MoS2 graphene  oxide  (rGO)  nanocomposite  is  proposed.  The  possible  mechanism  to  this phase  transformation  was  investigated  using  different  spectroscopy  techniques,  and supported  by  density  functional theory  theoretical  calculations.  A  mixture  of  the  1T'and 2H-MoS2 phases was observed from the Raman and Mo 3d High Resolution X-ray photoelectron (HRXPS) spectra analysis in the MoS2-rGO nanocomposite. After surface decoration with gold nanoparticles the concentration of the 1T' phase decreases making evident a phase transformation. According to Raman and valence band spectra analyses, the  AuNPs induces a p-type doping in MoS2-rGO nanocomposite. We proposed as a main  mechanism  to  the  MoS2  phase  transformation  the  electron  transfer  from  Mo 4dxy,xz,yz in  1T'  phase  to  AuNPs  conduction  band.  At  the  same  time,  the  unoccupied electronic structure was investigated from S K -edge Near Edge X-Ray Absorption Fine Structure (NEXAFS) spectroscopy. Finally, the electronic coupling between unoccupied electronic states was investigated by the core hole clock approach using Resonant Auger spectroscopy (RAS), showing that AuNPs affect mainly the MoS2 electronic states close to Fermi level.

## 1 INTRODUCTION

Over the past few years, two-dimensional transition metal dichalcogenides (TMDs) have become attractive options for electronic devices, transistors, biosensors, as well as for applications in catalysis and energy storage devices [1-3]. Among the TMD family MoS2 is the most investigated due to its unique physical and chemical properties [4,5]. A  singular  feature  of  MoS2  layered  materials  is  the  structural  polymorphism,  which modulates  its  electronic  structure.  In  particular,  the  2H  and  1T  phases  with  different arrangement of the S and Mo atoms have been reported for MoS2 crystals [6]. The 2HMoS2 is the most stable structure, where each layer is constructed from the Mo atom sandwiched between two S atoms in a trigonal prismatic (D3h) geometry. On the other hand,  the  1T-MoS2  phase  is  based  on  Mo  atoms  octahedrally  (Oh)  coordinated  to  S atoms. MoS2 in 1T phase is metastable (easily converted to the stable 2H phase) while in the octahedral distorted configuration (1T') it turns into a phasethat is thermodynamically stable [7]. The trigonal prismatic symmetry in 2H-MoS2 induces a semiconductor  electronic  structure  with  monolayer  direct  band  gap  of  ~1.8  eV,  [1,8] while the octahedral coordination of the Mo atoms in the 1T'-MoS2 phase gives rise to a metallic  behavior  with  good  conductivity  [1,9].  Recently,  several  works  about  the physical and chemical treatment of MoS2 to obtain a reversible transition between these two phases have been reported [6,10-12]. In most of them, the 1T'-MoS2 phase presents superior  electrocatalytic  properties,  while  2H-MoS2  is  an  excellent  candidate  for optoelectronic applications  [13-15].

While  isolated  MoS2  has  attractive  properties,  the  formation  of  MoS2-graphene nanocomposites could be an excellent approach to improve its performance for different device  applications  [16-20]  as  the  mechanical  flexibility,  electronic  conductivity  and chemical stability of graphene could added to the properties of isolated MoS2. Recently it  was reported that p-MoS2/n-rGO nanocomposites have better photocatalytic activity in  hydrogen  generation  when  compared  to  pristine  MoS2  [21,22].  At  the  same  time noble metal nanoparticles (NPs) decorating the MoS2-graphene nanocomposite surface could potentially extend its functionalities as novel catalytic, magnetic, and optoelectronic nanomaterials even further [2,23-26]. Among these nanoparticles, Gold (AuNPs) is of special interest due to their non-toxicity and excellent stability. In fact, Au-MoS2 composite synthesis, electrical and thermal properties and its application on photocatalytic water splitting and hydrogen production has been the subject of a number of works [27-31].

Nevertheless,  the  knowledge  of  the  electronic  structure  of  the  MoS2-graphene nanocomposites  is  a  crucial piece of information  for better understanding  their biosensing,  photonics,  catalytic  and  optoelectronic  device  performance.  In  particular, controlling  the  different  phases  with  metallic  and  semiconductor  behavior  of  the nanocomposite  is  of  utmost  importance  for  appropriately  tailoring  properties,  and subsequent  applications.  In  this  sense,  in  the  present  work,  the  effect  of  AuNPs decoration on the stability of MoS2 (1T' and 2H) phases and in the electronic structure of a MoS2-rGO nanocomposite was investigated. The local electronic structure of either the pristine nanocomposite,  and  decorated  with  AuNPs  was  studied  using  High Resolution X-ray Photoelectron Spectroscopy (HRXPS), Near Edge X-Ray Absorption Fine Structure (NEXAFS), Resonant Auger Spectroscopy (RAS), and Density Functional Theory simulations (DFT). The non-local electronic structure was investigated by Valence band and Raman spectra. A mixture of the 1T' and 2H phases of  MoS2  was  observed  from  the  Raman  spectrum  in  the  solvothermal-synthesized MoS2-rGO nanocomposite and corroborated from Mo 3d HRXPS spectra analysis. A

decrease  of  the  Mo 4+ (1T')  species  is  shown  after  surface  decoration  with  AuNPs, making  evident  a  phase  transformation  from  1T'  to  2H-MoS2.  We  identify  surface electron transfer processes from MoS2-rGO to AuNPs as the main mechanism for this phase transformation using Raman and XPS valence band spectra analysis. At the same time,  the  unoccupied  electronic  structure  was  investigated  from  S  K-edge  NEXAFS spectroscopy. The degree of delocalization and/or electronic coupling between unoccupied electronic states was investigated by the core hole clock approach showing that AuNPs affect the electronic states close to the Fermi level.

## 2. EXPERIMENTAL DETAILS

## 2.1 Synthesis procedure

Graphene oxide synthesis was carried out by a modified Hummers method in a calorimetric automated reactor. 0.75 g of pristine graphite flakes (Aldrich) was added to 90 mL of sulfuric acid (Sigma-Aldrich) e 10 ml of phosphoric acid followed by the slow addition of 4.5 g of potassium permanganate. This system was kept under stirring for two hours at 50 C. Subsequently, the temperature was decrease for 0 C then poured on o o 400ml  of  ice,  followed  by  2  mL  of  hydrogen  peroxide  (30  vol%  on  water,  SigmaAldrich). The solid material was purified by centrifugation and washed with different amounts of water, hydrochloric acid solution (10 vol%), ethanol, acetone and DI water again. The black and solid material (Graphite oxide - Gr-O) was dried under vacuum overnight. An aqueous suspension of graphite oxide was then sonicated (50W, 40 kHZ) in  DI  water  for  2  min.  The  resulting  brown  and  stable  suspension  was  found  to  be Graphene Oxide.

For  the  preparation  of  MoS2-rGO  nanocomposite,  25 mg  of  (NH4)2MoS4  was added  to  10 mg  of  graphene  oxide  (GO)  dispersed  in  10 ml  of  dimethylformamide (DMF). The mixture was sonicated at room temperature for approximately 10 min until a clear and homogeneous solution was achieved. After that, 0.1 ml of N2H4·H2O was added. The reaction solution was further sonicated for 30 min before transferred to a 150  mL  Teflon-lined  autoclave.  The  autoclave  was  sealed  and  heated  in  an  oven  at 200 °C for 10 h. The product was collected by centrifugation at 8000 rpm for 5 min and resuspended  in  DI  water.  This  washing  process  was  repeated  5  times  to  remove  the DMF.

Gold  nanoparticles  were  synthesized  according  the  procedure  described  by Grasseschi et al [32]. All glassware were previously cleaned with aqua regia (3HCl:1HNO3),  in  order  to  prevent  any  possible  influence  of  contaminants  in  gold reduction  process.  The  synthesis  was  performed,  by  heating  50  mL  of  gold  solution HAuCl4 solution (5.08 x 10 -4 mol L - 1 ) in a 125 mL round bottom flask, and refluxing, using a computer controlled system, for keeping the temperature (± 1°C) and stirring rates constants. Then, 1.7 mL of aqueous sodium citrate solution (0.038 mol L -1 )  was added dropwise (100 µLs -1 ),  while  the  mechanical stirring and temperature were kept constant, at 1150 rpm and 95°C, respectively. After 5 min, the solution was cooled to room temperature.

A  simple  method  was  utilized  to  obtain  the  MoS2-rGO-AuNPs  nanocomposite. Thin  film  of  MoS2-rGO  was  deposited  on  the  SiO2/Si  substrate  by  the  drop  casting method. After that, two drops of 25μL of the AuNPs solution were deposited to cover the entire film surface. The sample was dried in air at room temperature for 24 h.

## 2.2 Characterization

In order  to  obtain  morphological  information  of  the  samples,  transmission electron microscopy (TEM, JEOL  JEM  2100), Scanning transmission electron microscopy (STEM) using a high angular dark field detector (HAADF, FEI Titan 80300) and Scanning electron microscopy (SEM, JEOL JSM-7800F and Phenom ProX) were  performed.  The  Raman  spectra  were  collected  using  a  WITec  Alpha  300R confocal Raman imaging microscope using a laser line centered at 532 nm and 0.508 mW of  power.  For  reducing  the  sample  locations  effect,  the  Raman  spectra  in  both samples were collected at four different points and the reproducibility of results were observed. X-ray photoelectron spectroscopy (XPS)  (K-Alpha  Thermo  Scientific)

measurements and analyses were conducted to investigate the local electronic structure of  the  chemical  species  on  MoS2-rGO  and  MoS2-rGO-AuNPs  nanocomposites.  The monochromatized Al Kα (hν=1486.6 eV) excitation energy with 400 μm X-ray spot size was used for XPS measurements. The electron energy analyzer was operated at constant pass  energy  of  25  eV,  and  200  eV  for  high  resolution  (HR)  and  survey  spectra, respectively. An instrumental energy resolution of 0.25 eV determined from Ag5/2 peak from pure silver was used for HRXPS experiments. A flood gun source of low energy electrons  and  Ar   ions  was  used  during  all  measurements  in  order  to  prevent  surface + charging.  The  high-resolution  XPS  spectra  were  processed  using  Thermo  Scientific's Avantage  XPS  software  package  (version  4.61)  and  using  a  linear  combination  of Gaussian and Lorentzian line shapes for the spectra fitting, with a Shirley function for background correction. The binding energy scale was calibrated by attributing an energy value of 284.5 eV to C-C/C-H species in HR C1s spectrum.

The electronic structure for unoccupied states was investigated from X-ray absorption (XAS)  and  Resonant  Auger  (RAS)  spectroscopies  experiments.  XAS  and  RAS  were measured at the soft X-ray spectroscopy (SXS) beamline at the Brazilian Synchrotron Light Source (LNLS) facilities [33]. A Si(111) double-crystal monochromator in high resolution condition with energy bandwidth of 0.48 eV was used to cover Sulphur Kedge.  Near  Edge  X-Ray  Absorption  Fine  Structure  spectra  were  recorded  in  the  total electron yield mode (TEY). The final data was normalized by this photon flux spectrum (estimated  from  Au  mesh)  to  correct  the  fluctuations  in  beam  intensity.  Presented spectra are averages from at least three scans, background corrected by a linear pre-edge subtraction  and  linear  regression  beyond  the  edge.  Multiple-scan  RAS  spectra  were collected inside an ultrahigh vacuum chamber (UHV) with a base pressure of 10 -9 mbar using  a  hemispherical  electron  energy  analyzer  (Specs  model  phoibos  150)  with  45º

take-off  direction  of  Auger  electrons  and  25  eV  of  pass  energy.  The  total  energy resolution  was  0.76  eV.  RAS  spectra  fittings  were  performed  using  Pseudo-Voigt profile functions (linear combination of Gaussian (G) and Lorentzian (L) functions) and the background was corrected using a Shirley function.

## 2.3 Theoretical Simulations

Plane-wave density functional theory [34,35] was used to obtain the electronic ground-state using the Perdew-Burke-Ernzerhof (PBE) generalized gradient exchangecorrelation functional, [36] implemented in the Quantum-Espresso (QE) package, [37] and  Non-empirical  van  der  Waals  corrections  proposed  by  Tkachenko  and  Scheffler [38] were included in all calculation. The kinetic energy cutoff was set to 90 Ry and a mesh of 14 x 14 x 1 k-points in the Monkhorst-Pack scheme was used. The structures were fully optimized to their equilibrium positions with forces smaller than 0.01 eV/Å. A vacuum region of 15 Å was used to suppress the coupling between neighboring slabs. The  interfaces  were  modeled  by  choosing  an  Au  (111)  surface  with  4  atomic  layers. Subsequently  a  fully  relaxed  1T'-MoS2 (2H-MoS2)  monolayer  is  adsorbed  on  the Au(111) surface following the arrangement proposed by Zhou et al [39]. By doing this, both the Au(111) and 2H-MoS2 unit cell is matched with the ideal lattice constant of 1T'-MoS2 monolayers. We should mention that this five-layer model has been adopted in previous works describing well some features observed in experiments [40,41].

## 3. RESULTS AND DISCUSSION

The morphology of the MoS2-rGO and MoS2-rGO-AuNPs nanocomposites were characterized by SEM, TEM e STEM microscopy images and are depicted in Figure 1. . As  seen  in  SEM  (Figure  1a),  TEM  (Figure  1b)  and  STEM  (Figure  1c)  images,  the MoS2-rGO  nanocomposite  consist  of  MoS2  layer  covering  the  surface  of  the  rGO sheets.  MoS2  basal  planes  are  clearly  observed  from  high  magnification  TEM  image shown  in  Figure  1b.  Moreover,  the  HRTEM  image  reveals  a  large  number  of  MoS2 layers  with  interlayer  distance  of  0.62  nm  (corresponding  to  the  (002)  plane)  stacked together.  Energy  dispersive  X-ray  spectra  (EDX)  (Figure  1g  and  Figure  S1  on  the Supporting Information File (SI)) shows that Mo, S, C and O elements were distributed uniformly on the entire flake. Some regions show the formation of spherical particles of MoS2 with an average diameter of approximately a hundred nanometers covering the rGO surfaces (Figure S1).

The effect of AuNPs decorating the MoS2-rGO surface is presented in Figure 1d, showing a substantial coverage of AuNPs (bright points) in the surface of the MoS2 and promoting the formation wrinkled nanosheets. The TEM and STEM images on Figure 1e and f show that the AuNPs are spherical with an average size of 23.5 ± 3.5 nm with good  size  dispersion,  as  indicated  by  the  size  distribution  on  Figure  1h.  The  EDX spectra record at different points (Figure 1g and Figure S1 and S2) confirm the presence of gold on the MoS2-rGO surface.

Figure 1. SEM images of MoS2-rGO (a) and MoS2-rGO-AuNPs (d) nanocomposites. TEM images  of  MoS2-rGO  (b)  and  MoS2-rGO-AuNPs  (e)  nanocomposites.  STEM  HAADF  images  of  MoS2-rGO  (c)  and  MoS2-rGO-AuNPs  (f)  nanocomposite.  EDX spectra of MoS2-rGO and the MoS2-rGO-AuNPs nanocomposites of the selected areas on c and f (g). AuNPs size distribution (h).

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00854v1-figure-b1adfdc3-a8be-4db0-b9db-0dc1c15a0733.jpg)

Figure  2  shows  the  Raman  spectra  of  MoS2-rGO  and  MoS2-rGO-AuNPs nanocomposites.  These  spectra  exhibit  the  D,  G  and  D´  peaks,  vibrational  modes characteristic  of  graphitic  materials  [39,42].  The  G-band  corresponds  to  the  in-plane optical  mode  due  to  bond  stretching  of  graphitic  sp   carbon  atoms.  The  D-band 2 originates  from  the  lattice  defect  and  lattice  distortion,  while  D´-band  is  attributed  to inter and intra-valley scattering processes. The three peaks observed at 327, 379.1 and 407  cm -1 (Figure.  2(b))  correspond  to  the  in-plane  E1g and  E2g 1 and  out-plane  A1g vibrational modes of the 2H-MoS2, respectively [42-44]. The A1g peak position and the A1g-E2g 1 frequency difference (~28 cm -1 ) point to the formation of few-layer MoS2 with more than 5 layers [45]. A blue shift of about ~1 and 4 cm -1 (Fig.  2(c))  after  AuNPs surface decoration were observed for E2g 1 and A1g Raman modes of MoS2, respectively. The last behavior is an indicative of involvement of charge transfer processes between MoS2-rGO  sheets  and  dispersed  AuNPs,  more  specifically  a  p-type  doping,  where electrons are transferred from MoS2-rGO to AuNPs [46]. Other three peaks at 150, 218 and  328  cm -1 ,  attributed  to  the  J 1 ,  J 2 and  J 3 longitudinal  acoustic  modes  of  S-Mo-S bonds  in  1T'-MoS2  phase,  are  characterizing  the  Raman  spectrum  of  the  MoS2-rGO nanocomposite (Figure 2(b)). Demonstrating the coexistence of 1T' and 2H phases in this sample [7,47]. The coexistence of this two phase in MoS2-rGO nanocomposite was also  reported  by  Jeffery  et  al.,  showing  that  1T'  phase  stability  is  associated  to  rGO content [48]. After AuNPs surface decoration the intensity of J1, J2 and J3 peaks of 1T' phase becomes much weaker, while the A1g peak (typical of 2H-MoS2 phase) becomes more intense. This result is an indication of phase transformation from metallic 1T' to the  semiconducting  2H-MoS2  phase  with  the  presence  of  AuNPs.  The  metallic  to semiconductor transformation in MoS2-rGO  nanocomposite  after  AuNPs  surface decoration  could  be  a  promising  approach  to  keep  the  light  absorbing  properties  of MoS2 with a good electrical conductivity, mechanical stability and high surface area due to  the  presence  of  rGO  support,  making  this  material  an  excellent  candidate  for optoelectronic devices and photocatalytic applications.

Figure 2. (a) Raman spectra of the MoS2-rGO and MoS2-rGO- AuNPs nanocomposites. (b) Raman spectra showing the MoS2 peak regions (inside of red rectangle in figure (a)). (c) Raman spectra showing E2g 1 and A1g vibrational modes (inside of blue rectangle in figure (b)).

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00854v1-figure-c66a4552-16f3-4f1f-85bf-8bb9589a5849.jpg)

The chemical composition of the MoS2-rGO and MoS2-rGO-AuNPs nanocomposites was estimated from survey XPS spectra as shown in Figure 3. The core level Mo 3d, S2p, C1s and O1s peaks found in the spectrum of MoS2-rGO confirm the presence  of  the  constituent  elements  in  this  nanocomposite.  Additionally,  Au  4f  core level doublet peaks (Au 4f7/2 at 84.1 eV and Au 4f5/2 at 87.8 eV shown in Figure S3) are observed for the MoS2-rGO-AuNPs  sample, confirming the presence of gold nanoparticles in metallic state decorating the MoS2-rGO surface. The atomic percentages for each nanocomposite are reported on Table 1. The S/Mo atomic ratio of ~2, close to the theoretical stoichiometry formula of MoS2 is found for pristine MoS2rGO. However, a significant decrease  (from 17.1% in pristine MoS2-rGO to 8.3% in MoS2-rGO-AuNPs) in the S content is observed after AuNPs surface decoration. The last result may be associated to the fact that the AuNPs on the MoS2-rGO surface are adsorbed  on  top  of  the  S  atoms  sites.  This  result  is  in  agreement  with  previous theoretical  reports  where  was  found  that  Au  adatom  favors  to  adsorb  at  the  top  of  S atom and with a strong hybridization between the s orbital of Au and the Mo 4d states [49,50]. A slight increase of C and O species content is also observed in the MoS2-rGOAuNPs sample compared with the pristine case, which can be associated to the presence of citrate ligands utilized to stabilize the AuNPs in solution [32].

Figure 3 . XPS survey spectra of MoS2-rGO and MoS2-rGO-AuNPs nanocomposites.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00854v1-figure-63afdab0-6bdd-4766-96a5-d5a84f23a35b.jpg)

Table  1 .  Surface  chemical  composition  (at.%)  distribution  of  MoS2-rGO  and  MoS2rGO-AuNPs nanocomposite films obtained from XPS survey spectra analysis .

|                  |   C1s |   O1s |   Mo3d |   S2p | Au4f   |
|------------------|-------|-------|--------|-------|--------|
| MoS 2 -rGO       |  55.4 |  19.6 |    7.8 |  17.1 | -      |
| MoS 2 -rGO-AuNPs |  57.5 |  24.4 |    9   |   8.3 | 0.73   |

AuNPs doping effects in the stability of MoS2 (1T' and 2H) phases and in the local electronic structure for the MoS2-rGO nanocomposite were investigated with high resolution  XPS  spectra  analysis.  Figure  4  shows  the  C1s,  S2p,  Mo  3d  and  O1s  high resolution  XPS  spectra  of  both  nanocomposites.  The  fitting  parameters,  (Binding Energy - BE), full width at half maximum (FWHM) and species amount (% area) of high resolution spectra are summarized in the Table S1. The high resolution C1s XPS spectra of both nanocomposites showed in Figure 4(a) were deconvoluted using three components: peak at BE=284.5 eV can be attributed to C-C/C=C sp  carbon species, the 2 peak  at  BE=285.9  eV  can  be  attributed  to  hydroxyl  carbon  C-O,  and  the  peak  at BE=288.2  eV  carboxylate  carbon  O-C=O  [25].  These  spectra  are  similar  to  the  C1s XPS spectrum of isolated rGO reported in the literature [25,28]. There are no significant differences between  the  C1s  XPS  spectrum  of  MoS2-rGO  before  and  after  the decoration with AuNPs.

Three sulphur species with their respective spin-orbital doublets are observed in the S2p XPS spectra of both nanocomposites (Figure 4(b)). The peaks at BE = 161.8 eV and 163.1 eV correspond to the S 2p3/2 and 2p1/2 sulfur species in MoS2 [51-53]. The second S species observed in the S2p region was attributed to bridging C-S-C structures (BE = 163.3  eV  and  164.4  eV  to  the  S  2p3/2  and  2p1/2,  respectively)  [35].  The  high energy  component  at  BE = 168.5  eV  (S  2p3/2)  can  be  associated  to  S 6+ species  in  CSOX-C sulfate groups [52,53].

More representative differences between the electronic structure of MoS2-rGO and MoS2-rGO-AuNPs nanocomposites are observed in the high resolution Mo 3d and O1s  XPS  spectra.  According  to  previous  reports  the  diverse  electronic  properties  of TMDs arise from the progressive filling of the non-bonding d bands [54,55]. The effect of chalcogen atoms on the electronic structure is minor compared with that of the metal atoms, since the top of the valence band has higher contribution from the Mo orbitals. The  phase  stability  of  TMDs  also  depends  of  the  effective  change  in  the  d-electron count in the transition metal atom.

The Mo 3d XPS spectrum of MoS2-rGO nanocomposite is characterized by four contributions associated to different oxidization states and structural phases of the Mo species in this nanocomposite (Figure 4(c)). The peaks at BE = 230.0 eV and 233.2 eV correspond to Mo 4+ 3d5/2 and Mo 4+ 3d3/2 components of 2H-MoS2 (2H) phase of MoS2. The  deconvolution  of  the  Mo  3d  spectrum  identified  additional  peaks  (Mo 4+ 3d5/2  at 229.0 eV and Mo 4+ 3d3/2 232.1 eV) appearing at BE ~1 eV below of the corresponding peaks of the 2H phase which were attributed to 1T'-MoS2 phase [10,51,52,56-60]. The peaks at 231.2 and 234.4 eV, with separation energy of 3.2 eV, can be attributed to the Mo 3d5/2 and Mo 3d3/2 due to the presence of Mo 5+ [43,53]. In the high energy region of the  spectrum,  the  Mo  3d5/2  (232.7  eV)  and  Mo  3d3/2  (235.8  eV)  peaks  associated  to Mo 6+ can be found [52, 53]. The peak at BE = 226.3 eV in the low energy region of the Mo  3d  spectrum  corresponds  to  S2s  contribution.  The  Mo3d  HRXPS  results  are  in accordance  with  the  Raman  discussion,  showing  that  MoS2-rGO  nanocomposite  is composed of a mix of 1T' and 2H MoS2 phases. The same Mo chemical species are observed for the MoS2-rGO-AuNPs sample; however, some important differences are seen concerning their content after AuNPs surface decoration. We notice an increase of Mo 6+ oxidation species, while the Mo 4+ (1T')/ Mo 4+ (2H) ratio decreases from 1.7 to 0.6 after  the  decoration  of  the  MoS2-rGO  surface  with  Au  nanoparticles.  The  increase  of Mo 6+ and the decrease of Mo 4+ (1T'-MoS2) can be interpreted as electron transfer from MoS2-rGO to Au NPs, converting the MoS2-rGO electronic structure from a metallic to a  semiconductor  character,  corroborating  with  our  Raman  spectroscopy  results.  The increment of Mo 6+ in MoS2 after AuNPs decoration was also reported by Kim et al. and was attributed to oxidation of MoS2 to molybdic acid [61].

The  high  resolution  O1s  spectrum  (Figure  4(d)  bottom)  was  deconvoluted  by  three peaks at BE=  530.6, 531.7 and 533.1eV,  respectively. These  contributions are associated  with  C-C=O,  C=O/-COOH  and  OH  groups,  respectively.  After  decorating the MoS2-rGO surface with AuNPs, the OH species disappear, which may be attributed to a reduction of the surface adsorbed oxygen (water).

Figure 4 . High resolution XPS  spectra of MoS2-rGO  and MoS2-rGO-AuNPs nanocomposites: (a) C1s, (b) S2p, (c) Mo 3d and (d) O1s core levels.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00854v1-figure-2df5dcb2-71e5-4afb-b89c-10b14c0e7d30.jpg)

To elucidate the mechanism that induces the phase transition in the nanocomposite, DFT calculations were performed on the different MoS2 phases with or without the presence of gold. It has been proposed that a phase transition can be induced by  charge  transfer  to  the  TMD  [58].  According  to  Gao,  et  al.,  electron  injection  can stabilize  the  1T'-MoS2  phase  [58].  However,  our  experimental  results  show  that electrons are transferred from the MoS2 to the AuNPs reducing the stability of the 1T'phase and enabling the transition to the more stable 2H-MoS2. We looked at the effects of the interaction between Au and MoS2 in the electronic structure (Figure 5(b)). For the 2H phase adsorbed on an Au (111) surface (see Figure S4) we note little or no effect on the band structure of MoS2 compared to the isolated case. On the other hand, for the 1T'-phase - which is metallic - there is a strong interaction between the metal and the monolayer of MoS2, particularly around the G and M points of the spectrum where the band character becomes intertwined between gold and the TMD indicating a stronger interaction which favors the electrons transfers between the AuNPs and MoS2.

Figure 5 . (a) Top and lateral view of the 1T' phase of MoS2 adsorbed on a gold (111) surface.  (b)  Band  structure  projected  on  orbitals  of  the  different  constituents  for  the isolated (1T'-MoS2 and Au (111)) structures (outer panels), and the composite material (inner panel).

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00854v1-figure-d0284554-7fb7-478c-ac81-804cb1724f9b.jpg)

The valence band (VB) XPS spectra of MoS2-rGO and MoS2-rGO-AuNPs nanocomposites are shown in Figure 6. The valence band spectrum for MoS2-rGO is qualitatively  similar  to  MoS2  stemming  from  the  hybridization  of  Mo4d  and  S3p electronic  states  [61].  According  to  crystal-field  theory,  Mo  4d  orbitals  are  split  into three orbitals (see the Figure  6(c)): one  with  low  energy 4𝑑𝑧 2 4d, two  doubly degenerated  composed  by 4𝑑𝑥 2 -𝑦 2 ,𝑥𝑦 4d(empty)  and  two  doubly  degenerated  4dxz,yz (empty) for 2H-MoS2 phase (in hexagonal D3h configuration). In this case Mo 4𝑑𝑧 2 is fully  occupied  by  two  spin  paired  electrons  forming  the  VB.  However,  1T'-MoS2 (octahedral  Oh (1T')) is  composed by three degenerated orbitals 4dxy, xz,yz and doubly degenerated 4𝑑𝑥 2 -𝑦 2 ,𝑧 2 VB  in  1T'-MoS2  is  composed  by  partially  occupied  4dxy,xz,yz [61,  62].  The  main  effect  of  AuNPs  surface  decoration  is  observed  through  the decreasing  of  the  peak  at  ~  2  eV,  close  to  valence  band  edge.  This  behavior  can  be associated to an  electron  transfer  from  Mo  4d  states  to  AuNPs  conduction  band  how was depicted from Mo3d HRXPS and Raman spectra analyzed previously. Therefore, after a careful analysis of the valence band region and from theoretical calculations by DFT, comparing the electronic coupling between Au and MoS2 states for 1T' and 2H phases (Figure 5(b) and Figure S4) we can conclude that a possible mechanism for the phase  transformation  from  1T'  to  2H-MoS2  that  arises  after  surface  decoration  is  the output of electrons specifically from the Mo 4dxy,xz,yz that make up the VB in phase 1T'.

Figure  6(b)  shows  the  extrapolation  procedure  to  determine  the  valence  band maximum edge for both nanocomposites from valence band XPS spectra. A shift ~ 0.1 eV  to  lower  BE  values  is  observed  after  nanoparticle  decoration.  This  shift  is  an indicative of p-type doping, where the AuNPs behave as electron acceptors from MoS2rGO valence band [61,62]. This result is in agreement with Mo3d XPS analysis where the electron transfer from MoS2-rGO to AuNPs decreased their metallic character.

Figure  6 . (a) Valence  band  XPS  spectra  of  MoS2-rGO  and  MoS2-rGO-AuNPs nanocomposites. (b) Extrapolation procedure to determine the valence band maximum level.  The inset show the electronic configuration induced by crystal-field splitting of octahedral Oh(1T')  and D3h(2H) MoS2 phases.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00854v1-figure-6a9e79bc-ab2c-4292-8d20-cf92879a84b5.jpg)

The  partially  unoccupied  states  were  investigated  with  S K -edge  NEXAFS spectroscopy. Figure 7 shows the S K -edge NEXAFS spectra of MoS2-rGO and MoS2rGO-AuNPs  nanocomposites.  The  MoS2-rGO  NEXAFS  spectrum  shows  two  main peaks below the sulfur ionization energy. Peak 2 (2471 eV) at resonance maximum can be attributed,  according  to  previous  reports,  [63-65]  to  electronic  transitions  from  the S1s  core  level  to  unoccupied  hybridized  S3p-Mo4d  electronic  states.  The  pre-edge shoulder at 2468.5 eV (peak 1) can be associated with the presence of S-O bond species [52,60,66].  A  third  peak,  located  at  2472.1  eV  and  attributed  to  S1s-3pz  electronic transitions has been observed for the MoS2 monolayer sample (black line spectrum in Figure 7) showed here as comparison [63,65].  However, peak 3 is poorly defined in the NEXAFS spectra of MoS2-rGO and MoS2-rGO-AuNPs nanocomposites. According to

Guay et al., the energy separation between S3px,y and S3pz electronic states is due to the difference of  their symmetric properties at symmetry points Γ and A of the Brillouin zone  for  the  2H-MoS2  phase  [65].  Considering  the  Mo3d  XPS  results  we  saw  that MoS2-rGO  nanocomposites  are  a  mixture  between  2H-MoS2  and  1T'-MoS2  phases, then, the presence of 1T'-MoS2 metallic phase changes the symmetry properties of S2p electronic states and reduces the energy separation between S3px,y and S3pz.

Figure 7. S K -edge NEXAFS spectra of MoS2-rGO (blue solid line) and MoS2-rGOAuNPs (red solid line) nanocomposites. The S K -edge NEXAFS spectrum of the MoS2 monolayer  obtained  by  CVD  [63]  (black  line)  is  also  shown  for  the  purpose  of comparison. The inset shows a zoom of the first resonance peak. The numbers indicate the photon energies used to obtain the S-K L2,3L2,3 RAS spectra.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00854v1-figure-81c3b2bd-f282-4a60-918c-6646836ee471.jpg)

The  degree of delocalization or electronic coupling between unoccupied electronic states is investigated by the core hole clock approach using S-K L2,3L2,3 RAS spectra. A detailed explanation about core hole clock method can be found elsewhere [67, 68] and is summarized in the supporting information file (SI). In this approach, the charge  transfer  times,  used  as  a  quantitative  measure  of  electronic  coupling  (lower charge  transfer  time  means  high  electronic  coupling),  are  determined  using  lifetime

(τCH=1.27 fs in the case of the S K -edge [69]) of the core electron hole as an internal reference clock by:

τCT=(IRaman/ICT-Auger)× τCH, whereIRaman and ICT-Auger represent the intensities of different core-hole decay channels achieved  by  S-K  L2,3L2,3  RAS  spectroscopy.  The  'Raman'  and  'CT-Auger'  electron decay channels correspond to different electronic final states.  Raman decay correspond to the spectator two hole and one electron final states (2h1e) where the excited electron does not participate in the decay process. The second CT-Auger decay process consists of two holes (2h) in the valence band, reached when the electron is transferred out of the atom  during  the  core-hole  lifetime.  S-K  L2,3L2,3  RAS  spectra  shown  in  Figure  8  are convoluted by these core-decay channels. The attribution of 'Raman' and 'CT-Auger' decay channels in the RAS spectra is based on their behavior when the incident photon energy  is  tuned  across  the  core  excitation  resonance.  In  Raman  decay  channels,  the kinetic energy of the emitted electron increases when the energy of an incident photon is tuned across the resonance, while the CT-Auger contribution keeps at constant kinetic energy independently of the energy of the incident  photon.    The  identification  of  the Raman and CT-Auger contributions forming the S-K L2,3L2,3 RAS spectra for MoS2 was reported recently by Garcia-Basabe et al [63]. According to the last mentioned behavior of the 'Raman' and 'CT-Auger' decay channels (showed in Figure S5), we identified two spectators (blue and green in Figure 8) and one CT-Auger (red) contributions.

In this way, we determined τCT for S-K L2,3L2,3 RAS spectra obtained at photon energies labelled as 1 (2468.5 eV), 2 (2471 eV) and 3 (2472.1 eV) in the inset of Figure 7.  The  excitation  of  an  electron  to  an  unoccupied  electronic  state  in  the  pre-edge shoulder of the S1s resonance spectrum (labelled as 1 (hυ=2468.5 eV)), the τCT of 5.38 ±  0.60  fs  and  7.74  ±  0.70  fs  were  obtained  for  MoS2-rGO  and  MoS2-rGO-AuNPs nanocomposites, respectively. The increase in the τCT value for this photon energy was due  to  a  decrease  of  the  CT-Auger  contribution  from  18%  in  MoS2-rGO  to  12%  in MoS2-rGO-AuNPs  nanocomposite.  On  the  other hand, for electrons excited to electronic states in the S K -edge resonance maximum (labelled as 2 (hυ=2471.0 eV)) the contribution of CT-Auger decay channel decrease from 24% to 17%, while the SP1 decay  channel  increases  from  56%  to  64%  after  AuNPs  decoration.  Therefore,  for excitation energy of 2471.0 eV the τCT increase from 3.67 ± 0.60 fs in the MoS2-rGO to 5.52 ± 0.70 fs in the MoS2-rGO-AuNPs nanocomposites. The increase of τCT observed in  the  MoS2-rGO-AuNPs  nanocomposite  can  be  interpreted  as  a  reduction  of  the metallic  character  of  the  MoS2-rGO  nanocomposite  due  to  the  AuNPs.  However,  for photon  energies  labelled  as  3  (hυ=2472.1  eV),  the  τCT  are  very  similar  for  both nanocomposites, close to 2.90 fs. The last results mean that the AuNPs affects only the unoccupied  electronic  states  near  to  the  MoS2-rGO  Fermi  level.  Thus,  the  results obtained by the core hole clock approach are in agreement with Mo 3d XPs analysis, where a transformation from metallic to semiconductor character after AuNPs decoration was observed.

![image](https://ac.marcodsn.me/arxiv-markdown-images/1908.00854v1-figure-2cce7547-fce3-4d8b-a780-dcc7180a274a.jpg)

Kinetic Energy (eV)

Figure 8 . SK L2,3L2,3 RAS spectra measured at photon energies labelled as 1-3 (2468.5 (a),  2471(b)  and  2472.1  eV  (c),  respectively)    in  S K -edge  NEXAFS spectrum. RAS spectra deconvolution in Raman spectators (blue - SP1 and green - SP2) and CT (red) decay channel are also showed.

## 4. CONCLUSION

In summary, we propose a simple approach to transform the MoS2 from metallic to semiconductor character by AuNPs  surface decoration in the solvothermal synthesized MoS2-rGO nanocomposite. The AuNPs induces a p-type doping in MoS2rGO nanocomposite and reduce the stability of 1T' phase favoring the transformation to 2H-MoS2. The main mechanism for this phase transition was electron transfer from 1T' Mo 4dxy,xz,yz  electronic  states  to  AuNPs  conduction  band.  The  unoccupied  electronic structure  is  also  affected  by  AuNPs  decoration,  showing  a  strong  electronic  coupling between AuNPs and MoS2 states close to the Fermi level. Our results suggest a practical method to modulate metallic and semiconductor character of MoS2 phases in MoS2-rGO nanocomposite.

## ASSOCIATED CONTENT

## Supporting Information

The SEM images and EDX spectra collected at different points in the MoS2-rGO and MoS2-rGO-AuNPs  nanocomposites,  Au  4f  HRXPS  spectrum  of  MoS2-rGO-AuNPs nanocomposite,  fitting  parameters  obtained  from  C1s,  O1s,  S2p  and  Mo3d  high resolution spectra deconvolution for the MoS2-rGO and MoS2-rGO-AuNPs nanocomposites, band structure projected on orbitals of the different constituents for the isolated  (2H-MoS2  and  Au  (111))  structures  and  the  composite  material,  Core  Hole Clock Approach description section and photon energy dependence of electron kinetic energy of Resonant Auger decay channels.

## ACKNOWLEDGEMENTS

- Y. Garcia-Basabe acknowledges to CNPq for financial support (project (nº408265/2016-7).  Research  partially  supported  by  LNLS  -  National  Synchrotron Light  Laboratory  (SXS-20160596)  and  by  CNPEM-LNNano  (XPS-21999),  Brazil. A.R.R. acknowledges financial support from CNPq and FAPESP  (Project nº 2012/50259-8)  and  the  Simons  Foundation  through  the  ICTP  Associateship  program. Theoretical calculations were carried out in the Scientific Computing Center at UNESP (NCC-Unesp), and in the Santos Dumont Supercomputer (LNCC-Santos Dumont).  D. Grasseschi acknowledges to FAPESP for the financial support (grant no. 2015/104053).

## References

- [1] Chhowalla,  M.,  Liu,  Z.,  Zhang  ,  H.  (2015)  Two-dimensional  transition  metal dichalcogenide (TMD) nanosheets Chem. Soc. Rev. 44 2584-2586.
- [2] Choi, W., Choudhary, N., Han, G.H., Park, J., Akinwande, D., Lee, Y.H. (2017) Recent  development  of  two-dimensional  transition  metal  dichalcogenides  and  their applications. Mater Today 20 116-129.
- [3] Lv, R., Robison, J.A., Schaak, R.E., Sun, D., Y., S., Mallouk, T.E., Terrones, M. (2015) Transition metal dichalcogenides and beyond: synthesis, properties, and applications of single- and few-layer nanosheets. Acc. Chem. Res. 48 56-64.
- [4] Barua,  S.,  Dutta,  H.S.,  Gogoi,  S.,  Devi,  R.,  Khan,  R.  (2018)  Nanostructured MoS2-Based Advanced Biosensors: A Review. ACS Appl. Nano Mater. 1 2-25.
- [5] Zhang, G., Liu, H., Qu, J., Li, J. (2016) Two-dimensional layered MoS2: rational design, properties and electrochemical applications Energy Environ. Sci. 9 1190-1209
- [6] Kan, M., Wang, J.Y., Li, X.W., Zhang, S.H., Li, Y.W., Kawazoe, Y., Sun, Q., Jena, P. (2014) Structures and Phase Transition of a MoS2 Monolayer. J. Phys. Chem. C 118 1515-1522.
- [7] Yu, Y., Nam, G.H., He, Q., Wu, X.J., Zhang, K., Yang, Z., Chen, J., Ma, Q., Zhao, M., Liu, Z., Ran, F.-R., Wang, X., Li, H., Huang, X., Li, B., Xiong, Q., Zhang, Q., Liu, Z., Gu, L., Du, Y., Huang, W., Zhang, H. (2018) High phase-purity 1T′-MoS2and 1T′-MoSe2-layered crystals. Nat. Chem. 10 638-643.
- [8] Mak,  K.F.,  Lee,  C.H.,  Hone,  J.,  Shan,  J.,  Heinz,  T.F.  (2010)  Atomically  thin MoS2: a new direct-gap semiconductor. Phys. Rev. Lett. 105 136805.
- [9] Wypych, F.,  Schöllhorn,  R.  (1992)  1T-MoS2,  a  new  metallic  modification  of molybdenum disulfide J. Chem. Soc., Chem. Commun. 19 1386-1388
- [10] Eda, G., Yamaguchi, H., Voiry, D., Fujita, T., Chen, M., Chhowalla, M. (2011) Photoluminescence from Chemically Exfoliated MoS2. Nano Lett 11 5111-5116.
- [11] Kappera,  K.,  Voiry,  D.,  Yalcin,  S.E.,  Branch,  B.,  Gupta,  G.,  Mohite,  A.D., chhowalla,  M.  (2014)  Phase-engineered  low-resistance  contacts  for  ultrathin  MoS2 transistors. Nat. Mater. 13 1128-1134.

[12] Scalise, E., Houssa, M., Pourtois, G., Afanas ev, V., Stesmans, A. (2012) StrainInduced  Semiconductor  to  Metal  Transition  in  the  Two-Dimensional  Honeycomb Structure of MoS2. Nano Res. 5 43-48.

- [13] Radisavljevic,  B.,  Radenovic,  A.,  Brivio,  J.,  Giacometti,  V.,  Kis,  A.  (2011) Single-layer MoS2 transistors. Nat. Nanotech. 6 147-150.
- [14] Tsai, M.-L., Su, S.-H., Chang, J.-K., Tsai, D.-S., Chen, C.-H., Wu, C.-l., Li, L.J., Chen, L.-J., He, J.-H. (2014) Monolayer MoS2 Heterojunction Solar Cells. ACS Nano 8 8317-8322.
- [15] Wang, Q.H., Kalantar-Zadeh, K., Kis, A., Coleman, J.N., Strano, M.S. (2012) Electronics  and  optoelectronics  of  two-dimensional  transition  metal  dichalcogenides. Nature Nanotech. 7 699-712
- [16] Chekin, F., Boukherroub, R., Szunerits, S. (2017) MoS2/reduced graphene oxide nanocomposite for sensitive sensing of  cysteamine in presence of uric acid in human plasma. Mater. Sci. Eng., C 73 627-632.
- [17] Chekin, F., Teodorescu, F., Coffinier, Y., Pan, G.-H., Barras, A., Boukherroub, R., Szunerits, S. (2016) MoS2/reduced graphene oxide as active hybrid material for the electrochemical detection of folic acid in human serum. Biosens. Bioelectron. 85 807813
- [18] Wang,  R.,  Gao,  S., Wang,  K., Zhou,  M., Cheng,  S., Jiang, K. (2017) MoS2@rGO Nanoflakes as High performance Anode Materials in Sodium on Batteries. Sci. Rep. 7 7963.
- [19] Xiang, Q., Yu, J., Jaroniec, M. (2012) Synergetic Effect of MoS2 and Graphene as Cocatalysts for Enhanced Photocatalytic H2 Production Activity of TiO2 Nanoparticles. J. Am. Chem. Soc. 134 6575-6578
- [20] Zhao, Y., Zhang , X., Wang, C., Zhao, Y., Zhou, H., Li, J., Jin, H. (2017) The synthesis  of  hierarchical  nanostructured  MoS2/Graphene  composites  with  enhanced visible-light photo-degradation property. Appl. Surf. Sci. 412 207-213.
- [21] Meng,  F.,  Li,  J.,  Cushing,  S.K.,  Zhi,  M.,  Wu,  N.  (2013)  Solar  Hydrogen Generation by Nanoscale p-n Junction of p-type Molybdenum  Disulfide/n-type Nitrogen-Doped Reduced Graphene Oxide. J. Am. Chem. Soc. 135 10286-10289.
- [22] Ren, X., Ren, X., Pang, L., Zhang, Y., Ma, Q., Fan, H., Liu, S.F. (2016) MoS2 /sulfur  and  nitrogen  co-doped  reduced  graphene  oxide  nanocomposite  for  enhanced electrocatalytic hydrogen evolution. Int. J. Hydrogen Energy 41 916-923
- [23] Bai,  L.,  Cai,  X.,  Lu,  J.,  Li,  L.,  Zhong,  S.,  Wu,  L.,  Gong,  P.,  Chen,  J.,  Bai,  S. (2018)  Surface  and  Interface  Engineering  in  Ag2S@MoS2  Core-Shell  Nanowire Heterojunctions for Enhanced Visible Photocatalytic Hydrogen Production. ChemCatChem 10 2107 -2114
- [24] Choi,  M.,  Koppala,  S.K.,  Yoon,  D.,  Hwang,  J.,  Kim,  S.M.  (2016)  A  route  to synthesis  molybdenum  disulfide-reduced  graphene  oxide  (MoS2-RGO)  composites using supercritical methanol and their enhanced electrochemical performance for Li-ion batteries. J Power Sources 309 202-211.
- [25] Li,  X.,  Li,  J.,  Zhou,  X.,  Ma,  Y.,  Zheng,  Z.,  Duan,  X.,  Qu,  Y.  (2014)  Silver nanoparticles  protected  by  monolayer  graphene  as  a  stabilized  substrate  for  surface enhanced Raman spectroscopy. Carbon 66 : 713-719.
- [26] Zhang  ,  S.,  Wang,  L.,  Zeng,  Y.,  Xu,  Y.,  Tang,  Y.,  Luo,  S.,  Liu,  Y.,  Liu,  C. (2016)  CdS-Nanoparticles-Decorated  Perpendicular  Hybrid  of  MoS2  and  N-Doped Graphene  Nanosheets  for  Omnidirectional  Enhancement  of  Photocatalytic  Hydrogen Evolution ChemCatChem 8 2557-2564.
- [27] Huang,  X.,  Zhen,  Z.,  Bao,  S.,  Wang,  M.,  Qi,  X.,  Fan,  Z.,  Zhang,  H.  (2013) Solution-phase  epitaxial  growth  of  noble  metal  nanostructures  on  dispersible  singlelayer molybdenum disulfide nanosheets. Nat Commun 4 1444.
- [28] Shi, Y., Huang, J.-K., Jin, L., Hsu, Y.-T., Yu, S., F., Li, L.-J., Yang, H.Y. (2013) Selective  Decoration  of  Au  Nanoparticles  on  Monolayer  MoS2  Single  Crystals. Sci. Rep. 3 1839.
- [29] Yin, Z., Chen, B., Bosman, M., Cao, X., Chen, J., Zheng, B., Zhang, H. (2014) Au  Nanoparticle-Modified  MoS2  Nanosheet-Based  Photoelectrochemical  Cells  for Water Splitting. small 10 3537-3543.
- [30] Cho,  Y.,  Sohn,  A.,  Kim,  S.,  Hahm,  M.G.,  Kim,  D.-H.,  Cho,  B.,  Kim,  D.-W. (2016) Influence of Gas Adsorption and Gold Nanoparticles on the Electrical Properties of CVD-Grown MoS2 Thin Films. ACS Appl. Mater. Interfaces 8 21612-21617.
- [31] Sreeprasad,  T.S.,  Nguyen,  P.,  Kim,  N.,  Berry,  V.  (2013)  Controlled,  DefectGuided,  Metal-Nanoparticle  Incorporation  onto  MoS2  via  Chemical  and  Microwave Routes: Electrical, Thermal, and Structural Properties. Nano Lett. 13 4434-4441.
- [32] Grasseschi, D., Ando, R.A., Toma, H.E., Zamarion, V.M. (2015) Unraveling the nature  of  Turkevich  gold  nanoparticles:  the  unexpected  role  of  the  dicarboxyketone species. RSC Adv. 5 5716-5724
- [33] Abbate, M., Vicentin, F.C., Compagnon-Cailhol, V., Rocha, M.C., Tolentino, H. (1999) The Soft X-ray Spectroscopy Beamline at the LNLS: Technical Description and Commissioning Results. J. Synchrotron Radiat. 6 964-972.
- [34] Hohenberg, P., Kohn, W. (1964) Inhomogeneous electron gas. Phys. Rev. 136 B864-B871.
- [35] Kohn, W., Sham, L.J. (1965) Self-consistent equations including exchange and correlation effects. Phys. Rev. 140 A1133-1138.
- [36] Perdew, J.P., Burke, K., Ernzerhof, M. (1996) Generalized gradient approximation made simple. Phys.Rev.Lett. 77 3865-3868.
- [37] Giannozzi,  P.,  Baroni,  S.,  Bonini,  N.,  Calandra,  M.,  Car,  R.,  Cavazzoni,  C., Ceresoli, D., Chiarotti, G.L., Cococcioni, M., Dabo, I. (2009) QUANTUM ESPRESSO: a  modular  and  open-source  software  project  for  quantum  simulations  of  materials. J. Phys.: Condens. Matter 21 395502.
- [38] Tkatchenko,  A.,  Scheffler,  M.  (2009)  Accurate  Molecular  Van  Der  Waals Interactions from Ground-State Electron Density and Free-Atom Reference Data. Phys. Rev. Lett. 102 073005.
- [39] Zhou, Y., Kiriya, D., Haller, E.E., Ager III, J.W., Javey, A., Chrzan, D.C. (2016) Compliant substrate epitaxy: Au on MoS2. Phys. Rev. B 93 054106.
- [40] Bruix, A., Miwa, J.A., Hauptmann, N., Wegner, D., Ulstrup, S., Grønborg, S.S., E.,  S.C.,  Dendzik, M., Cabo, A.G., Bianchi, M., Lauritsen, J.V., Khajetoorians, A.A., Hammer,  B.,  Hofmann,  P.  (2016)  Single-layer MoS2  on  Au  (111):  Band gap renormalization and substrate interaction. Phys. Rev. B 93 165422.
- [41] Yan,  Z.,  Chen,  L.,  Yoon,  M.,  Kumar,  S.  (2016)  The  Role  of  Interfacial Electronic  Properties  on  Phonon  Transport  in  Two-Dimensional  MoS2  on  Metal Substrates. ACS Appl. Mater. Interfaces 8 33299-33306.
- [42] Ferrari,  A.C.  (2007)  Raman  spectroscopy  of  graphene  and  graphite:  Disorder, electron-phonon coupling, doping and nonadiabatic effects. Solid State Commun. 143 47-57.
- [43] Cheng,  C.-K.,  Lin,  C.-H.,  Wu,  H.-C.,  Ma,  C.C.M.,  Yeh,  T.-K.,  Chou,  H.-Y., Tsai, C.-H., Hsieh, C.-K. (2016) The Two-Dimensional Nanocomposite of Molybdenum  Disulfide  and  Nitrogen-Doped  Graphene  Oxide  for  Efficient  Counter Electrode of Dye-Sensitized Solar Cells. Nanoscale Res Lett 11 117.
- [44] Windom,  B.C.,  Sawyer,  W.C.,  Hahn,  D.W.  (2011)  A  Raman  Spectroscopic Study of MoS2 and MoO3: Applications to Tribological Systems. Tribol Lett 42 301310.
- [45] Lee, C., Yan, H., Brus, L.E., Heinz, T.F., Hone, J., Ryu, S. (2010) Anomalous Lattice Vibrations of Single-and Few-Layer MoS2. ACS Nano 4 2695-2700.

[46] Chakraborty,  B.,  Bera,  A.,  Muthu,  D.V.S.,  Bhowmick,  S.,  Waghmare,  U.V., Sood,  A.K.  (2012)  Symmetry-dependent  phonon  renormalization  in  monolayer  MoS2 transistor. Phys. Rev. B 85 161403.

- [47] Wang, S., Zhang, D., Li, B., Zhang, C., Du, Z., Yin, H., Bi, X., Yang, S. (2018) Ultrastable In-Plane 1T-2H MoS2 Heterostructures for Enhanced Hydrogen Evolution Reaction. Adv. Energy Mater. 8 1801345.
- [48] Jeffery,  A.A.,  Rao,  S.R.,  Rajamathi,  M.  (2017) MoS2-reduced graphene oxide (rGO) hybrid paper for catalytic applications by simple exfoliation-costacking. Carbon 112 8-16.
- [49] Wu, P., Yin, N., Li, P., Cheng, W., Huang, M. (2017) Adsorption and diffusion behaviors of noble metal adatoms (Pd, Pt, Cu, Ag and Au) on MoS2 monolayer: a firstprinciples study. . Phys. Chem. Chem. Phys. 19 20713-20722.
- [50] Ju, W., Li, T., Su, X., Li, H., Li, X., Ma, D. (2017) Au clusters adsorption on the perfect and the defective MoS2 monolayers: structural and electronic properties. Phys. Chem. Chem. Phys. 19 20735-20748.
- [51] Ambrosi,  A.,  Sofer,  Z.,  Pumera,  M.  (2015)  2H→1T  phase  transition  and hydrogen evolution activity of MoS2, MoSe2, WS2 and WSe2 strongly depends on the MX2 composition. Chem. Commun. 51 8450-8453
- [52] Cai, L., He, J., Liu, Q., Yao, T., Yan, W., Hu, F., Jiang , Y., Zhao, Y., Hu, T., Sun, Z., Wei, S. (2015) Vacancy-Induced Ferromagnetism of MoS2 Nanosheets. J. Am. Chem. Soc. 137 2622-2627.
- [53] Dai,  X.,  Du,  K.,  Li,  Z.,  Sun,  H.,  Yang,  Y.,  Zhang,  W.,  Zhang,  X.  (2015) Enhanced hydrogen evolution reaction on few layer MoS2  nanosheet secoated functionalized carbon nanotubes. Int. J. Hydrogen Energy 40 8877-8888
- [54] Chhowalla, M., Shin, H.S., Eda, G., Li, L.-J., Loh, K.P., Zhang, H. (2013) The chemistry of two-dimensional layered transition metal dichalcogenide nanosheets. Nat. Chem. 5 263-275.
- [55] Pandey,  M.,  Bothra,  P.,  Pati,  S.K.  (2016)  Phase  Transition  of  MoS2  Bilayer Structures. J. Phys. Chem. C 12 3776-3780.
- [56] Acerce,  M.,  Voiry,  D., Chhowalla,  M.  (2015)  Metallic  1T  phase  MoS2 nanosheets as supercapacitor electrode materials. Nat. Nanotech. 10 313.
- [57] Fan,  X.,  Xu,  P.,  Zhou,  D.,  Sun,  Y.,  Li,  Y.C.,  Nguyen,  M.A.T.,  Terrones,  M., Mallouk, T.E. (2015) Fast and Efficient Preparation of Exfoliated 2H MoS2 Nanosheets

by  Sonication-Assisted  Lithium  Intercalation  and  Infrared  Laser-Induced  1T  to  2H Phase Reversion. Nano Lett 15 5956-5960.

- [58] Gao,  G.,  Jiao,  Y.,  Ma,  Y.,  Jiao,  Y.,  Waclawik,  E.,  Du,  A.  (2015)  Charge Mediated  Semiconducting-to-Metallic  Phase  Transition in Molybdenum  Disulfide Monolayer and Hydrogen Evolution Reaction in New 1T′ Phase. J. Phys. Chem. C 119 13124-13128.
- [59] Lin,  L.,  Miao,  N.,  Wen,  Y.,  Zhang,  S.,  Ghosez,  P.,  Sun,  Z.,  Allwood,  D.A. (2016) Sulfur-depleted monolayered molybdenum disulfide nanocrystals for superelectrochemical hydrogen evolution reaction. ACS Nano 10 8929-8937.
- [60] Yang, S., Zhang , K., Wang, C., Zhang, Y., Chen, S., Wu, C., Vasileff, A., Qiao, S., Song,  L.  (2017)  Hierarchical  1T-MoS2  Nanotubular  Structures  for  Enhanced Supercapacitive Performance. J. Mater. Chem. A 5 23704-23711.
- [61] Liang, K.S., Hughes, G.J., Chianelli, R.R. (1984) UPS investigation of poorly crystallized MoS2. J. Vac. Sci. Technol. A 2 991.
- [62] Tao,  J.,  Chai,  J.W.,  Zhang,  Z.,  Pan,  J.S.,  Wang,  J.  (2014)  The  energy-band alignment at molybdenum disulphide and high-k dielectrics interfaces. Appl. Phys. Lett. 104 232110.
- [63] Garcia-Basabe, Y., Rocha, A.R., Vicentin, F.C., Villegas, C.E.P., Nascimento, R.,  Romani,  E.C.,  de  Oliveira,  E.C.,  Fechine,  G.J.M.,  Li,  S.,  Eda,  G.,  Larrude,  D.G. (2017) Ultrafast charge transfer dynamics pathways in two-dimensional MoS2graphene  heterostructures:  a  core-hole  clock  approach Phys.  Chem.  Chem.  Phys. 19 29954-29962.
- [64] Li, D., Bancroft , G.M., Kasrai, M., Fleet, M.E., Feng, X.H., Tan, K.H. (1995) Polarized  X-ray  Absorption  Spectra  and  Electronic  Structure  of  Molybdenite  (2HMoS2). Phys Chem Minerals 22 123-128.
- [65] Guay,  D.,  Divigalpitiya,  W.M.R.,  Bélanger,  D.,  Feng,  X.H.  (1994)  Chemical Bonding in Restacked Single-Layer MoS2 by X-ray Absorption Spectroscopy. Chem. Mater. 6 614-619.
- [66] Yang, C.-Y., Chiu, K.-C., Chang, S.-J., Zhang, X.-Q., Liang, J.-Y., Chung, C.S., Pan, H., Wu, J.-M., Tseng, Y.-C., Lee, Y.-H. (2016) Phase-driven magneto-electrical characteristics of single-layer MoS2. Nanoscale 8 5627-5633.
- [67] Föhlisch, A., Feulner, P., Hennies, F., Fink, A., Menzel, D., Sanchez-Portal, D., Echenique,  P.M.,  Wurth,  W.  (2005)  Direct  observation  of  electron  dynamics  in  the attosecond domain. Nature 436 373-376.

[68] Menzel, D. (2008) Ultrafast charge transfer at surfaces accessed by core electron spectroscopies. Chem. Soc. Rev. 37 2212-2223.

- [69] Campbell,  J.L.,  Papp,  T.  (2001)  Widths  of  the  Atomic  K-N7  Levels. Atomic Data and Nuclear Data Tables 77 1-56.
Yunier Garcia-Basabe Gabriela F. Peixoto Daniel Grasseschi Eric C. Romani Flávio C. Vicentin Cesar E. P. Villegas Alexandre. R. Rocha Dunieskys G. Larrude
Phase Transition and Electronic Structure Investigation of MoS$_2$-rGO Nanocomposite Decorated with AuNPs
In this work a simple approach to transform MoS$_2$ from its metallic (1T' to
semiconductor 2H) character via gold nanoparticle surface decoration of a
MoS$_2$ graphene oxide (rGO) nanocomposite is proposed. The possible mechanism
to this phase transformation was investigated using different spectroscopy
techniques, and supported by density functional theory theoretical
calculations. A mixture of the 1T'- and 2H-MoS2 phases was observed from the
Raman and Mo 3d High Resolution X-ray photoelectron (HRXPS) spectra analysis in
the MoS$_2$-rGO nanocomposite. After surface decoration with gold nanoparticles
the concentration of the 1T' phase decreases making evident a phase
transformation. According to Raman and valence band spectra analyses, the AuNPs
induces a p-type doping in MoS$_2$ -rGO nanocomposite. We proposed as a main
mechanism to the MoS$_2$ phase transformation the electron transfer from Mo
4d-xy,xz,yz in 1T' phase to AuNPs conduction band. At the same time, the
unoccupied electronic structure was investigated from S K-edge Near Edge X-Ray
Absorption Fine Structure (NEXAFS) spectroscopy. Finally, the electronic
coupling between unoccupied electronic states was investigated by the core hole
clock approach using Resonant Auger spectroscopy (RAS), showing that AuNPs
affect mainly the MoS2 electronic states close to Fermi level.